Mixed Cations and Structural Complexity in (Eu1-xCax)4In3Ge4 and (Eu1-xCax)3In2Ge3-The First Two Members of the Homologous Series A2[n+m]In2n+mGe2[n+m] (n,m= 1, 2, ...\ιnfty; A = Ca, Sr, Ba, Eu, or Yb)
Tae-Soo You; Paul H. Tobash; Svilen Bobev; Inorganic Chemistry 49 (2010) 1773–1783; doi:10.1021/ic902144h

data_4314833
_publ_section_title
;
 Mixed Cations and Structural Complexity in (Eu1-xCax)4In3Ge4 and
 (Eu1-xCax)3In2Ge3-The First Two Members of the Homologous Series
 A2[n+m]In2n+mGe2[n+m] (n,m= 1, 2, ...\\infty; A = Ca, Sr, Ba, Eu, or Yb)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1773
_journal_page_last               1783
_journal_paper_doi               10.1021/ic902144h
_journal_volume                  49
_journal_year                    2010
_chemical_formula_moiety         'Ca1.40 Eu2.60 Ge4 In3'
_chemical_formula_sum            'Ca1.4 Eu2.6 Ge4 In3'
_chemical_formula_weight         1086.03
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.631(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   17.0124(17)
_cell_length_b                   4.5559(10)
_cell_length_c                   7.5403(4)
_cell_measurement_reflns_used    911
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      36.74
_cell_measurement_theta_min      2.51
_cell_volume                     556.97(14)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHEMXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.934
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0511
_diffrn_reflns_av_sigmaI/netI    0.0437
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            4206
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         30.74
_diffrn_reflns_theta_min         2.51
_exptl_absorpt_coefficient_mu    31.666
_exptl_absorpt_correction_T_max  0.0425
_exptl_absorpt_correction_T_min  0.0256
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    6.472
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       bar
_exptl_crystal_F_000             933
_exptl_crystal_size_max          0.045
_exptl_crystal_size_mid          0.035
_exptl_crystal_size_min          0.030
_refine_diff_density_max         1.977
_refine_diff_density_min         -1.606
_refine_diff_density_rms         0.356
_refine_ls_extinction_coef       0.00024(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         911
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.093
_refine_ls_R_factor_all          0.0461
_refine_ls_R_factor_gt           0.0334
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0202P)^2^+0.5041P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0586
_refine_ls_wR_factor_ref         0.0626
_reflns_number_gt                740
_reflns_number_total             911
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic902144h_si_002_1.cif
_cod_data_source_block           Eu2.60Ca1.40In3Ge4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_original_formula_sum        'Ca1.40 Eu2.60 Ge4 In3'
_cod_database_code               4314833